### Ames Laboratory Accepted Manuscripts

### Ames Laboratory

### 2-5-2019

### Ultrafast manipulation of topologically enhanced

### surface transport driven by mid-infrared and

### terahertz pulses in Bi2Se3

### Liang Luo

*Iowa State University and Ames Laboratory*, liangluo@iastate.edu

### Xu Yang

*Iowa State University and Ames Laboratory*, xuy@iastate.edu

### X. Liu

*University of Notre Dame*

### Zhiyan Liu

*Iowa State University and Ames Laboratory*, zyliu@iastate.edu

### Chirag Vaswani

*Iowa State University and Ames Laboratory*, chiragv@iastate.edu

**See next page for additional authors**

### Follow this and additional works at:

### https://lib.dr.iastate.edu/ameslab_manuscripts

### Part of the

### Condensed Matter Physics Commons

### , and the

### Quantum Physics Commons

This Article is brought to you for free and open access by the Ames Laboratory at Iowa State University Digital Repository. It has been accepted for inclusion in Ames Laboratory Accepted Manuscripts by an authorized administrator of Iowa State University Digital Repository. For more information, please contactdigirep@iastate.edu.

### Recommended Citation

Luo, Liang; Yang, Xu; Liu, X.; Liu, Zhiyan; Vaswani, Chirag; Cheng, Di; Mootz, M.; Zhao, Xin; Yao, Yongxin; Wang, Cai-Zhuang; Ho,
Kai-Ming; Perakis, I. E.; Dobrowolska, M.; Furdyna, J. K.; and Wang, Jigang, "Ultrafast manipulation of topologically enhanced surface
transport driven by mid-infrared and terahertz pulses in Bi2Se3" (2019).*Ames Laboratory Accepted Manuscripts*. 245.

### Ultrafast manipulation of topologically enhanced surface transport driven

### by mid-infrared and terahertz pulses in Bi2Se3

**Abstract**

### Topology-protected surface transport of ultimate thinness in three-dimensional topological insulators (TIs) is

### breaking new ground in quantum science and technology. Yet a challenge remains on how to disentangle and

### selectively control surface helical spin transport from the bulk contribution. Here we use the mid-infrared and

### terahertz (THz) photoexcitation of exclusive intraband transitions to enable ultrafast manipulation of surface

### THz conductivity in Bi2Se3. The unique, transient electronic state is characterized by frequency-dependent

### carrier relaxations that directly distinguish the faster surface channel than the bulk with no complication from

### interband excitations or need for reduced bulk doping. We determine the topological enhancement ratio

### between bulk and surface scattering rates, i.e.,

*γ*

### BS/

*γ*

### SS ~3.80 in equilibrium. The ultra-broadband,

### wavelength-selective pumping may be applied to emerging topological semimetals for separation and control

### of the protected transport connected with the Weyl nodes from other bulk bands.

**Keywords**

### Terahertz optics, Topological insulators, Ultrafast photonics

**Disciplines**

### Condensed Matter Physics | Quantum Physics

**Authors**

### Liang Luo, Xu Yang, X. Liu, Zhiyan Liu, Chirag Vaswani, Di Cheng, M. Mootz, Xin Zhao, Yongxin Yao,

### Cai-Zhuang Wang, Kai-Ming Ho, I. E. Perakis, M. Dobrowolska, J. K. Furdyna, and Jigang Wang

### ARTICLE

### Ultrafast manipulation of topologically enhanced

### surface transport driven by mid-infrared and

### terahertz pulses in Bi

_{2}

### Se

_{3}

### L. Luo

1### , X. Yang

1### , X. Liu

2### , Z. Liu

1### , C. Vaswani

1### , D. Cheng

1### , M. Mootz

3### , X. Zhao

1### , Y. Yao

1### , C.-Z. Wang

1### ,

### K.-M. Ho

1### , I.E. Perakis

3### , M. Dobrowolska

2### , J.K. Furdyna

2### & J. Wang

1Topology-protected surface transport of ultimate thinness in three-dimensional topological insulators (TIs) is breaking new ground in quantum science and technology. Yet a challenge remains on how to disentangle and selectively control surface helical spin transport from the bulk contribution. Here we use the mid-infrared and terahertz (THz) photoexcitation of exclusive intraband transitions to enable ultrafast manipulation of surface THz conductivity in Bi2Se3. The unique, transient electronic state is characterized by frequency-dependent carrier relaxations that directly distinguish the faster surface channel than the bulk with no com-plication from interband excitations or need for reduced bulk doping. We determine the topological enhancement ratio between bulk and surface scattering rates, i.e.,γBS/γSS~3.80 in equilibrium. The ultra-broadband, wavelength-selective pumping may be applied to emerging topological semimetals for separation and control of the protected transport connected with the Weyl nodes from other bulk bands.

https://doi.org/10.1038/s41467-019-08559-6 **OPEN**

1_{Department of Physics and Astronomy and Ames Laboratory-U.S. DOE, Iowa State University, Ames, Iowa 50011, USA.}2_{Department of Physics, University}

of Notre Dame, Notre Dame, IN 46556, USA.3_{Department of Physics, University of Alabama at Birmingham, Birmingham, AL 35294-1170, USA.}

Correspondence and requests for materials should be addressed to J.W. (email:jgwang@ameslab.gov)

123456789

## T

he recent discovery of topology-protected charge trans-port of three-dimensional (3D) TIs has led to a pro-mising platform for exploring both fundamental topological quantum phenomena and technological applica-tions1–7. The emergent behaviors associated with this exotic state of matter, such as spin-locking, helical spin structure, topological invariant, chiral anomaly, and dissipationless cur-rents8–13, offer new perspectives for achieving transformational technological applications in spintronics and quantum sensing, computing, and communications3_{beyond the current }

tech-nological limit. One of the current frontiers for topological phenomena lies in the fundamental challenge of how to dis-entangle and manipulate symmetry-protected transport from bulk conduction. On one hand, development and optimization of hot electron transistors and modulators operating at ultra-high THz frequencies will signiﬁcantly beneﬁt from the direct probing of ultrafast THz charge transport on the surface and from a better understanding of the fundamental effects of topological spin-locking on carrier scattering. Although the existence of a helical Dirac spectrum has been well established in electrical transport14 and photoemission8,15,16, ultrafast control of THz helical spin transport is much less known. This is due, in part, to the limitations of conventional transport characterization methods that are incapable of probing frequency-dependent conductivity characterized by femtose-cond (fs) in time and THz in energy scales, especially with low frequency photon pumping17–19. On the other hand, in 3D TIs, the coexistence and mutual scattering of Dirac and bulk car-riers lead to an intertwined response. Despite recent observa-tions from static THz measurements of TI samples with signiﬁcantly reduced doping and defects20,21, it is still chal-lenging to selectively control the intrinsic surface dynamics from the bulk contribution for samples that exhibit uninten-tional doping into bulk states.

The transport properties of 3D TIs are determined by carriers
in narrowly gapped bulk bands and by gapless surface states
protected by the time-reversal symmetry. Although the
spin-momentum locking of Dirac electrons increases the conductivity
from atomically-thin surface states, its contribution can still be
masked by the high density carrier conduction in static transport
measurements, at either bulk or interface states, even inﬁlms with
tens of nm thickness. Consequently, very few experimental
techniques are capable of isolating and studying the intrinsic
topological transport on the surface, especially for high Fermi
energies. Sophisticated characterization and sample synthesis are
involved, e.g., anisotropic magneto-transport by adjusting
mag-netic ﬁeld directions14 _{and signi}_{ﬁ}_{cantly reduced doping and}

thickness by thin ﬁlm engineering20–29. There has been con-siderable progress yet with complications, e.g., limited applic-ability or difﬁculty in the interpretation. For example, intrinsic Dirac-cones could be contaminated with possible gap opening in very thin samples. The separation of surface and bulk/interface contributions to the static THz conductivity spectra has to rely on reduced doping.

Recently, ultrafast THz conductivity has been shown to be promising by providing time resolution able to distinguish the surface from the bulk responses after suddenly driving the system out-of-equilibrium28,30. However, the high photon frequency pumping at 1.55 eV used so far introduces interband excitations from valence to conduction and other high lying bands at both surface and bulk. Such coupling causes population transfer between surface and bulk bands and enhanced scattering between high-energy states. Selective mid-IR and THz pump-THz probe spectroscopy used in this work represent powerful and versatile tools that allow us to measure and control surface transport in TIs, even for Fermi levelEFinto the bulk bands.

We emphasize several strategic advantages of low frequency pumping scheme like ours, as illustrated in Fig. 1a. First, in

**a**

**b**

**d**
**c** _{20}

15

10

5

0

248 meV pump

*T = *300K

4 3 2 1 0 –1 –2

*t*gate(ps)
20

15

10

5

0

248 meV pump

*T = *5 K
–4
–2
0
2

Δ*E*_{sample} (a.u.)
25

20

15

10

5

0

10 8 6 4

Photon energy
(meV)
Static, *T *= 5 K

Exp Fit

–4 –3 –2 –1 0 1

10 8 6 4

Photon energy (meV) Exp Fit

1

(

)(10

–3

Ω

–1)

Δ

*t*pp

(ps)

Δ

*t*pp

(ps)

THz

probe Mid-IR& THz

pump

*E*

*E*F

*E*inter

k

1

(

)(10

3)

Fig. 1Ultrafast mid-IR/THz pump and THz probe spectroscopy for Bi2Se3.aSchematic of the surface and bulk electronic band structures of the Bi2Se3ﬁlm

with Fermi level (EF) indicated, illustrating mid-IR/THz intraband excitations and THz conductivity detection.bStatic THz spectra ofσ1(ω) andε1(ω) (red

dots) of the Bi2Se3ﬁlm atT=5 K. Shown together are the theoreticalﬁtting (gray lines) using the composite THz model from Eq. (1).c,dA 2D false-color

plot of pump-induced THzﬁeld changesΔEsampleas a function of gate timetgate(horizontal axis) and pump-probe delayΔtpp(vertical axis) after 248 meV

(5μm) photoexcitation of the sample atcT=300 K anddT=5 K, respectively. Plotted together are the corresponding static THzﬁeldsEsample(tgate)

(green curves) and their pump-induced changes_{Δ}_{E}sample(tgate) atΔtpp=1 ps (blue curves, ×5, from the cut positions as marked by the blue-dashed lines),

in order to compare their relative amplitude changes and phase shifts at different temperatures

### ARTICLE

NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-019-08559-6 [image:4.595.134.462.433.662.2]contrast to interband photoexcitation that couples high-energy electronic states between two bands, THz and mid-IR photo-excitation mainly excites intraband transitions nearEF. Here the photon energy is below the insulating bandgap and interband transition energy, which suppresses many other charge transfer channels. This allows measurement of intrinsic scattering rates and strongly constrains theﬁtting parameters to scattering rates only, as discussed later. Additionally, our time resolution can separate intrinsic surface from bulk conductivity via their dif-ferent hot carrier cooling times, i.e., resolve the issue directly in the time-domain. The extracted spectra fully characterize THz response functions as the complex frequency-dependent con-ductivity. In this way we can determine the intrinsic surface electron scattering rates and their ultrafast dynamics, compli-mentary to commonly used transport14, and photoemission8,16 measurements. Finally, comparison of the conductivity for wavelength-selective photoexcitations below and above the interband transition enabled by tuning the pump photon energy allows the optical control of carrier dynamics of surface and bulk bands in a selective way. However, in contrast to the several interband photoexcitation studies performed in TIs28,30, mid-IR, and THz pump-induced conductivity experiments have not been carried out so far in TIs.

Here we report ultrafast THz charge transport and dynamics in n-type Bi2Se3 that arise from nonequilibrium Dirac surface

and bulk transient states induced by intraband mid-IR and THz photoexcitation. We observe frequency-dependent carrier cooling times of photoinduced THz conductivity that clearly differentiate surface from bulk contributions and allow deter-mination of their scattering rates. We show that the topological enhancement of surface transport suppresses the surface elec-tron scattering rate as compared to the bulk, i.e.,γBS/γSS~3.80

in equilibrium. This result is consistent with surface helical spin transport in the presence of short-range disorder31. Moreover, the clear similarities between mid-IR and THz pumping and their distinct difference from high-photon-energy cases clearly show: (1) ultrafast manipulation of the surface and bulk THz conductivities via wavelength-selective pumping; (2) intraband vs. interband excitation mechanisms driven by low and high-photon-energy pumping. These are distinctly different from any known THz transport measure-ments so far, which have used either high-energy optical fre-quency photoexcitation or only detected time-averaged properties. The intraband, mid-IR/THz-induced THz con-ductivity provides a powerful method for isolating the surface transport channel in TIs—unhindered by complications from interband pumping or high density doping into bulk states. The distinct spectral-temporal characteristics obtained in this way in TIs may be extended to study and understand much broader topological phenomena32.

Results

Frequency-dependent dynamics of THz conductivity spectra. The Bi2Se3thinﬁlm sample, 50 nm thick, is grown by molecular

beam epitaxy on a 0.5 mm thick sapphire substrate. The static THz conductivity spectra are shown in Fig.1b. The details about THz data analysis, sample preparation, and experimental setup are described in the Methods. We characterize the none-quilibrium THz responses of the Bi2Se3thinﬁlm by extracting the

real parts of the transient conductivityσ1(ω,Δtpp) and dielectric

functionε1(ω,Δtpp) as a function of both the frequencyωand the

pump-probe delay time Δtpp. These spectra describe the dis-sipative and inductive parts of the response functions of quasi-particles, respectively, and are extracted from raw THzﬁelds in time-domain.

The pump-induced raw THz ﬁelds in Fig. 1c, d exhibit a distinctly different temperature dependence. At 300 K, the transmittedﬁeld changeΔEsamplehas a πphase shift relative to the static ﬁeld Esample without any other frequency- and time-dependent changes. This behavior is characteristic of an absorption-dominated response, i.e., a large increase in σ1(ω).

On the other hand, at low temperatureT=5 K, a large inductive response ε1(ω) appears in addition to the dissipative one, as

manifested by a signiﬁcant frequency- and time-dependent THz

ﬁeld reshaping besides the dominantπphase shift as in the 300 K case. These distinct spectral-temporal characteristics give rise to several salient features in the extracted THz response functions Δσ1(ω) andΔε1(ω), shown in Fig.2a–d, that allow us to directly

separate the intrinsic surface and bulk transport contributions to the conductivity from the experimental data withoutﬁtting.

Theﬁrst feature, shown in Fig.2a, b, is that the pump-induced THz conductivity spectra Δσ1(ω) extracted from the measured

time-dependent THzﬁelds exhibit a clear bipolar behavior with frequency-dependent cooling times under intraband excitation (248 meV) at low temperature (5 K). Speciﬁcally, as shown by comparing three time-cut spectra (white-dashed lines in Fig.2b), Δσ1(ω) at early times (Δtpp<5 ps) is characterized by a strong

bleaching, i.e., a negative conductivity change, in the low frequency 2–3 meV range. This changes to a strong absorption, i.e., positive conductivity change, towards high frequencies up to ~7 meV, as seen in the 1 ps trace (black dots in Fig. 2a). At Δtpp>5ps, the low frequency bleaching has quickly diminished, and the transient spectra are dominated by the high frequency absorption with longer cooling times, e.g., as shown in the 5.4 ps (red dots) and 15.4 ps (blue dots) traces. The frequency cuts of the Δσ1(ω) spectra from Fig.2b are summarized in Fig.2e (atω=2

meV) and2f (atω=7 meV) (black dots) as a function ofΔtpp. Clearly, the cooling times depend on the probe frequency, i.e., the faster (slower) cooling for ultrafast THz conductivity change at low (high) frequency. The characteristic cooling time for the 2 meV probe isτSS=1.48 ± 0.14 ps, signiﬁcantly shorter than that

for the 7 meV probeτBS=5.30 ± 0.18 ps (the uncertainty is from

single exponential ﬁtting). Such a frequency-dependent decay of THz electron transport is consistent with the signiﬁcant THz pulse reshaping seen in Fig.1d, which indicates more than one cooling channel of hot electrons.

Second, to understand these experimental results, we compare them with prior ultrafast THz responses from photoexcited Bi2Se3

samples. A decrease in their thickness has been shown to induce a
transition to a surface-like, pronounced bleaching behavior that
differs from a bulk-like, absorption one30_{. The latter is expected}

from the ionized impurity scattering in the bulk, which decreases
scattering rate after pumping at low temperatures33_{and gives rise}

to a positive Δσ1(ω) towards zero frequency (see below for

details). Therefore our results show that THz transport and dynamics of surface and bulk fermions can be selectively separated in time and measured by tuning probe frequency. Most intriguingly, upon closer scrutiny, the time-dependent scattering rates of surface Dirac (red line) and bulk (green line) fermions in Fig. 2e, f match very well with the conductivity dynamics at 2 meV and 7 meV, respectively. These scattering rates are extracted byﬁtting the time-dependent conductivity data as discussed later. This clearly shows that the experimentally obtainedΔσ1(ω) probed at 2 meV can be used to directly measure

surface transport dynamics, distinctly different from bulk conduction (at 7 meV), without reference to theoretical models. In between 2 and 7 meV, Δσ1(ω) dynamics consist of mixed

cooling time, as shown in Fig. 3. Strikingly, this high-temperature behavior is opposite to the low-high-temperature conductivity responses in Fig. 2. This is consistent with the different, raw THz ﬁeldsΔEsample between T=5 K and 300 K seen in Fig. 1c, d. Speciﬁcally, the pump-induced Δσ1(ω)

spectra at 300 K, shown as 2D false-color plot in Fig.3a, are all positive,Δσ1(ω) > 0, without the negative bleaching component

over the measured time and spectral range. Particularly,Δσ1(ω)

has similar amplitude at 5 K and 300 K as shown in Figs.2a and 3b, but Δε1(ω) at 300 K is decreased to approximately one

order of magnitude smaller than its counterpart at 5 K, as
shown in Figs.2c and3c (see also the Supplementary Note 1).
This indicates large photoinduced conductive response in
comparison with inductive one at the elevated temperature.
Since phonon-mediated coupling and charge transfer between
surface and bulk are activated above the Debye temperature at
182 K15_{, the dominance of positive} _{Δ}_{σ}

1(ω) at 300 K is

consistent with our conclusion that the bulk transport and surface-bulk charge transfer dominate at high temperatures and lead to the induced absorption. This suppresses the induced bleaching from the surface seen at 5 K in Fig.2a. On the other hand, the frequency-dependent cooling times previously seen at 5 K are no longer present at the elevated temperature. As shown in Fig. 3d the THz conductivities Δσ1(ω) at ω=2, 5, and 7 meV as a function of pump-probe

delayΔtpp, now decay with the same time at 300 K. The cooling time of ~4.8 ps is similar to the bulk state cooling time τBS

observed at 5 K. These observations corroborate again our claim that the low frequency conductivity at 2 meV, with faster cooling time observed at 5 K, comes from surface transport that is separated from the bulk channel. Furthermore, these distinct differences between high and low temperatures in ultrafast charge transport suggest that surface-bulk charge transfer in TIs is suppressed at low temperature.

20 15 10 5 0 1.0 0.5 0.0 2 meV 5 meV (×1.25) 7 meV (×1.32) 1.0 0.5 0.0 1 ps 5 ps 16 ps 20 15 10 5 0 8 7 6 5 4 3 2

Photon energy (meV)
*T *= 300 K
–1.0 0.0 1.0

1.0 0.5 0.0 8 6 4 2

Photon energy (meV)
1 ps
5 K
1 ps
300 K
**a** **b**
**c**
**d**
Δ
*t*pp
(ps)

Δ1 (10 –3 Ω–1 ) Δ 1 ( )(10 –3 Ω –1) Δ 1 ( )(10 –3 Ω –1 ) Δ 1 ( )(10 3)

Δ*t*pp(ps)

Fig. 3Frequency-independent dynamics of THz spectra at high

temperature.aPump-induced THz spectra of_{Δ}_{σ}1(ω) after 248 meV (5μm)

photoexcitation withﬂuence 12μJ cm−2atT=300 K as a function of pump-probe delayΔtpp.bTHz conductivityΔσ1(ω) from three cut positions

froma, at_{Δ}_{t}pp=1, 5, 16 ps, as indicated by the white-dashed lines.cTHz

spectra ofΔε1(ω) atΔtpp=1 ps for 5 K (gray dots) and 300 K (black dots),

the amplitude of which is much smaller at high temperature, opposite to low temperature ones in Fig.2c, d.dThe comparison of THz conductivity Δσ1(ω) at three frequencies: 2, 5, and 7 meV, as a function ofΔtpp(scaled

to match amplitude), from three frequency-cut positions fromaas
indicated by magenta, blue, and black dots, respectively. The
frequency-independent relaxation dynamics of_{Δ}_{σ}1(ω) indicates the strong coupling of

surface and bulk states that make them decay together at high temperature

Δ1 (2 meV)

Δ1 (7 meV) γSS γBS –1 0 1 ps 5.4 ps 15.4 ps 1 ps 5.4 ps 15.4 ps 15 10 5 0 7 6 5 4 3 2

Photon energy (meV)
*T *= 5 K
–1 0 1

7 6 5 4 3 2

Photon energy (meV)

1 0

*T *= 5 K
1
0
0.6
0.4
0.2
0.0
30
20
10
0
3.1
3.0
2.9
2.8
–1.0
–0.5
0.0
1.3
1.2

Scattering rate (THz)

1.1
1.0
0.9
0.8
**a**
**b**
**c**
**d**
**e**
**f**
Δ
1
(
)(10
–3
Ω
–1
)
Δ
1
(
)(10
–3
Ω
–1)
Δ
1
(
)(10
–3
Ω
–1)
Δ
1
(
)(10
3)
Δ
*t*pp
(ps)

Δ*t*pp(ps)
Δ1 (10

–3 _{Ω}–1_{)} _{Δ}

1 (10
3_{)}

Fig. 2Frequency-dependent dynamics of THz spectra at low temperature. Pump-induced THz spectra ofa,b_{Δ}_{σ}1(ω) andc,dΔε1(ω) after 248 meV (5μm)

photoexcitation withﬂuence 12μJ cm−2atT=5 K as a function of pump-probe delayΔtpp.aandcshow the THz spectra from three cut positions from the

corresponding 2D plots ofbandd, respectively, atΔtpp=1, 5.4, and 15.4 ps, as indicated by the white-dashed lines.eTHz conductivity at 2 meV, i.e.,

Δσ1(2 meV) (black dots, left axis), as a function ofΔtpp, from the frequency-cut position inbas indicated by the red-dashed line. The scattering rate of the

surface stateγSS(red curve, right axis) obtained from theoreticalﬁtting using Eq.1is plotted together to compare relaxation dynamics.fSimilar toe, THz

conductivity at 7 meV,Δσ1(7 meV) (black dots, left axis) and the scattering rate of bulk stateγBS(green curve, right axis) are plotted.Δσ1(7 meV) is from

the frequency-cut position inbas indicated by the green-dashed line. As shown clearly, the relaxation dynamics of the surface (bulk) scattering rate matches with that of THz conductivity at 2 meV (7 meV) very well. This frequency-dependent THz relaxation dynamics indicates surface (bulk) state is more sensitive to low (high) THz frequency

### ARTICLE

NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-019-08559-6 [image:6.595.122.479.49.270.2] [image:6.595.50.287.387.596.2]THz spectra analysis andﬁtting. To put these physical pictures on a strong footing, we quantitatively simulate the experimentally determined THz response functions Δσ1(ω) and Δε1(ω). By

extracting the temporal evolution of surface and bulk con-ductivity spectra, we obtain the intraband scattering rates and ultrafast dynamics of both Dirac (red line) and bulk (green line) fermions, as presented in Fig. 2e, f, respectively. A theoretical model consisting of contributions with Drude and Lorentzian lineshapes is used to reproduce the measured THz response functions. Speciﬁcally, two Drude terms account for surface state (SS) and bulk state (BS) plus one phonon oscillator centered at ω0~ 7.7 meV (1.9 THz),

~εðωÞ ¼ X j¼SS;BS

~εDrude

j ðωÞ þεphðωÞ ¼ε1

X

j¼SS;BS ðωpÞ2j

ω2_{þ}_{i}_{ωγ}

j

þ F

ðω0Þ2ω2iωΓ

;

ð1Þ

whereε∞is the background electrical permittivity and the plasma

frequency ðω2

pÞj¼ne2=ε0m is proportional to the density of

charge carriers of surface (nSS, j=SS) and bulk (nBS, j=BS) electrons.ωandeare the frequency and electron charge.ε0and m* are the vacuum electrical permittivity and carrier effective mass.γjis the scattering rate of surface (j=SS) and bulk (j=BS) carriers. In the last term of Eq.1,Fdenotes the effective transition strength of the optical phonon with resonance frequencyω0and

scattering rateΓ. Such a composite THz response model provides an excellent agreement with the pump-induced transient THz spectra over the entire measured pump-probe delays and spectral range as shown in Fig.4(cyan lines). Suchﬁt is achieved by only varying the scattering ratesγof surface and bulk carriers, i.e., the charge carrier densities of surface (nSS) and bulk (nBS) states remain constant in the ﬁts. Please also note that the optical phonon resonance ~7.7 meV is ﬁtted by F, ω0, and Γ of the

Lorentzian oscillator, which only affects locally the feature near

the resonance. Examples of typical ﬁts are shown in Fig. 4 at various time delays,Δtpp=1 ps, 9.4 ps, and 15.4 ps. The modelﬁt (cyan lines) is divided into the sum of the surface (green-dashed lines), bulk (blue-dashed lines), and phonon (magenta-dashed lines) responses. Detailed ﬁtting parameters are listed in the Supplementary Note 5.

We like to emphasize three key observations from the quantitative ﬁtting. First, while the static THz spectra, shown in Fig.1b, can be ﬁtted equally well with either single or multiple Drude components, the transient THz spectra, shown in Fig. 4, can only be ﬁtted by the two-Drude model. This is the case because the strong constraint imposed by the requirement to simultaneously describe both the conductivity Δσ1(ω) and the

dielectric function Δε1(ω) over broad temporal and spectral

ranges, shown in Fig.2a–d, instead of justﬁtting the lineshape as in the static case. Second, an even stronger constraint comes from the intraband, mid-IR/THz excitation scheme that most likely conserves the number of surface and bulk quasi-particles after the photoexcitation, i.e., carrier densities of both surface and bulk states are kept constant in the ﬁtting, ΔnSS=0 and ΔnBS=0 (more details and discussions in Fig. 5). Remarkably, by simply varying the surface and bulk scattering rates we are able to consistently reproduce the experimental results, as shown in Fig. 4, and extract the scattering rates (or inverse transport lifetimes that should not be confused with hot carrier cooling times)γSS(red line),γBS(green line), and their cooling dynamics

in Fig.2e, f. On theﬂip side, this excellent agreement implies that mid-IR/THz photoexcitation creates a unique nonequilibrium state of hot, yet mostly conserved, Dirac fermions and bulk carriers in their respective bands. Third, the equilibrium surface and bulk scattering rates, γSS and γBS extracted before the

photoexcitation, are 0.84 THz and 3.18 THz, respectively, which reveal an enhancement ratio,γBS/γSS~3.8. Remarkably, this value

matches very well with the topological enhancement factor, 4, for
protected, helical spin transport of non-interacting fermions in
the presence of short-range disorder such as structural defects
and surface or interface roughness. In the presence of long range,
Coulomb disorder, this enhancement decreases from 4 to 2 due to
increase of screening31_{. Furthermore, as shown in Fig.}_{2}_{e, f, the}

scattering rates of the surface Dirac and bulk fermions nearly coincide with the frequency-dependent decay of Δσ1(ω) for 2

meV and 7 meV probe, respectively. This corroborates again that tuning the THz probe frequency under mid-IR/THz pump can be used to disentangle the distinct symmetry-protected transport from the bulk conduction and measure their dynamics without reference to theoretical models. In between 2 and 7 meV, it consists of competing responses from surface and bulk, e.g., Δσ1(ω) at 3 meV consists of THz conductivity contributions from

both states with a similar strength.

Wavelength-selective pumping from THz to visible. Figure 5 highlights ultra-broadband, wavelength-selective pumping that extends from THz and mid-IR to near-IR and visible. This data show that our THz conductivities following 4 meV (Fig.5a) and 248 meV (Fig.5b) pump have similar bipolar lineshape. In con-trast, high-pump photon energy, e.g., 950 meV (Fig. 5d) and 1550 meV (Fig.5e), show an overall positive conductivity change down to 2 meV. The clear similarities between mid-IR and THz pumping and their distinct difference vs. high-energy pumping allow us to distinguish two excitation channels, i.e., intraband (interband) excitations with low (high) photon energy pumping. Importantly, the data obtained for THz and mid-IR pumping can be well-ﬁtted without changing carrier densities. In sharp con-trast, the data for high-photon-energy pumping cannot beﬁtted in this way. Speciﬁcally, our goodﬁttings obtained in Fig.5a, b –1

0

1 Δ*t*_{pp}_{ = 1 ps} Δ*t*pp = 9.4 ps Δ*t*pp = 15.4 ps

Exp Fitting Dirac Bulk Phonon 1.5 1.0 0.5 0.0 10 8 6 4 2 0.2 0.0 –0.2 0.2 0.1 0.0 –0.1 10 8 6 4 2

Photon energy (meV)
0.2
0.1
0.0
–0.1
–0.2
–0.05
0.00
0.05
10
8
6
4
2
**a**
**b**
**c**
**d**
**e**
**f**
Δ
1
(
)(10
–3
Ω
–1
)
Δ
1
(
)(10
3)

Fig. 4Theoreticalﬁtting of the pump-induced THz spectra.a,bTheﬁtting

ofΔσ1(ω) andΔε1(ω) for 248 meV (5μm) photoexcitation withﬂuence

12μJ cm−2atT=5 K and pump-probe delayΔtpp=1 ps. The experimental

results (red dots) areﬁtted very well by the THz model from Eq.1(cyan
lines), which consists of three individual components, i.e., the Dirac surface
state (green-dashed lines), bulk state (blue-dashed lines), and optical
phonon mode (pink-dashed lines). The_{ﬁ}tting results forc,d_{Δ}_{t}pp=9.4 ps

ande,fΔtpp=15.4 ps are plotted in the same manner asa,b

[image:7.595.54.290.184.235.2] [image:7.595.50.290.445.648.2]Exp Fitting Dirac Bulk Phonon

10 8 6 4 2 2

1

0

10 8 6 4 2 4

2

0

–2

–4

Δ

1

(

)(10

–3

Ω

–1)

Δ

1

(

)(10

3)

Δ*n*_{SS }= 0
Δ*n*_{BS }= 0

Δ*n*_{SS }= 0
Δ*n*_{BS }= 0

Δ*n*_{SS }= 0
Δ*n*_{BS }= 0

Δ*n*_{SS }= 0
Δ*n*_{BS }= 0

Δ*n*_{SS }= 0
Δ*n*_{BS }= 0

Δ*n*_{SS }> 0
Δ*n*_{BS }> 0
Δ*n*_{SS }> 0

Δ*n*_{BS }> 0
Frequency (meV)

10 8 6 4 2

Can NOT fit

10 8 6 4 2 10

8 6 4 2 248 meV pump

12 μJ cm–2 354 meV pump_{12 }_{μ}_{J cm}–2 1550 meV pump_{14 }_{μ}_{J cm}–2

10 8 6 4 2

Can NOT fit 950 meV pump

12 μJ cm–2

10 8 6 4 2 4 meV pump

180 kV cm–1

**a** **b** **c** **e**

**f** **g**

**d**

Frequency (meV)
Change density *n*

Fig. 5Ultrafast THz spectra by wavelength-selective pump from THz to visible. THz spectra for several pump photon energies:a4 meV,b248 meV,

c354 meV,d–f950 meV, ande,g1550 meV atΔtpp=1 ps. Figures forΔσ1andΔε1have the samexandyaxis ranges, respectively, for fair comparison.

The THz spectra fora4 meV,b248 meV, andc354 meV pump can be_{ﬁ}tted well by keeping the SS and BS carrier densities constant (_{Δ}_{n}SS=0 andΔnBS

=0) and only changing the scattering rates of SS and BS. However, the THz spectra cannot beﬁtted in the same way ford950 meV ande1550 meV pump. Instead, they have to beﬁtted by changing both the carrier densities (ΔnSS> 0 andΔnBS> 0) and the scattering rates of SS and BS, as shown in

fandg

### ARTICLE

NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-019-08559-6 [image:8.595.98.503.46.639.2]indicate that the pump-induced bulk components (dashed blue lines) have nearly identical amplitude and lineshape. This implies that the bulk responses following 4 meV and 248 meV pump are very similar, which indicate a possible transition from ﬁlled surface to empty bulk states following 248 meV pump cannot be a major channel, or at least any such contribution is much smaller in our probed THz spectral region than the main intraband sig-nals. Additionally, it is fully consistent that the negative surface response (dashed green lines) is greater following 4 meV pump than 248 meV and 354 meV pump (still below but closer to the bulk bandgap) in the linear Dirac dispersion. In strong contrast, for high-photon-energy pumping we can see that the THz con-ductivities are positive in the probe range and much larger. Importantly, they cannot be ﬁtted by the model with conserved carrier density any more, see Fig.5d, e. Instead, they can beﬁtted decently only withΔnSS> 0 andΔnBS> 0, as shown in Fig.5f, g. Their bulk (dashed blue lines) and surface (dashed green lines) components are both larger than their counterparts following low energy pump, which gives the overall positive THz conductivity change in the probed range, indicative of the bulk-dominant response. Moreover, please note that the ﬁttings are faithful, because it only needs to change two scattering rates, which leads to distinctly different THz lineshapes that uniquely converge. We also rule out the possibility that two different sets of scattering rates, which differ from each other by >2%, canﬁt the same data. These results clearly demonstrate the control of THz conductivity by ultra-broadband, wavelength-selective pumping from THz to visible.

Discussion

To highlight the difference between the intraband excitation scheme used in this work and the interband excitation found in previous literature, Fig.6a, b compare the ultrafast THz dynamics under 390 meV (3.18μm) and 248 meV (5μm) pumping, respectively. The former resonantly excites interband transitions in our bulk Bi2Se3sample (Fig.1a). Here, for simplicity, we show

the THzﬁeld changeΔEsamplebyﬁxing the gate timetgateat the peak of the static THz ﬁeld as a function of pump-probe delay Δtpp, similar to previous studies28,30. Unlike the above-obtained frequency-dependent conductivity Δσ1(ω) dynamics that closely

follows the pump-induced change of surface/bulk scattering rates,
ΔEsamplemeasured at aﬁxed gate time originates from
frequency-integrated responses within the measured spectral range ~2–10
meV. This frequency average leads to more complicated
dynamics that may come from all relaxation channels of opposite
signs as shown in Fig.2. Nevertheless, Fig.6shows that there is
still a distinct difference between the interband (Fig. 6a) and
intraband (Fig.6b) pump excitation schemes. On the one hand,
with resonant interband pump excitation at 390 meV (inset,
Fig.6a),ΔEsampleat several pumpﬂuences shows two main decay
features: (1) a dominant, fast overshoot, which exhibitsﬂ
uence-dependent amplitude and quickly diminishes within ~4 ps; (2) a
slow, hundreds of ps component, which is ﬂuence independent,
i.e., the ΔEsamplefor allﬂuences merge and decay together after
~100 ps. On the other hand, with intraband excitation at 248 meV
(inset, Fig.6b), the fast overshoot component is absent in the THz
responses at lowﬂuences≤12μJ cm−2_{, the}_{ﬂ}_{uence used for }

mid-IR pumping in Figs. 1–4. A distinct difference is clearly visible
between interband and intraband pumping with lowﬂuence, e.g.,
the 7μJ cm−2_{(cyan) and 9.5}_{μJ cm}−2_{(green) traces. Interestingly,}

increasing the mid-IR pump ﬂuence to 19μJ cm−2 (red line in Fig. 6b) leads to a transition to a decay proﬁle, where a fast overshoot component now appears similar to the interband photoexcitation, e.g., the 390 meV excitation scan at 1.6μJ cm−2 (pink line in Fig.6a). For a better comparison, this pink curve is also plotted in Fig.6b as aﬁlled gray curve, which resembles the 248 meV excitation scan at 19μJ cm−2, unlike for the lower ﬂ u-ences. This reveals the same relaxation mechanism between the two, which can be attributed to the two photon absorption (TPA) present in the high ﬂuence, mid-IR pumping case. This excites interband transitions in our sample in spite of below gap pump photon energy. The dynamics of Bi2Se3 under

high-photon-energy pumping have been extensively studied recently and the
few ps relaxation component is mainly from bulk-surface charge
transfer and/or decay that can give the overshoot feature after
interband carrier injection16_{. The absence of such process in the}

mid-IR pumping below ~12μJ cm−2 is consistent with the intraband excitation channel and its similarity with THz (few meV) pumping.

Although the optical transition from ﬁlled surface state to empty bulk state with 248 meV mid-IR pump is potentially allowed, our results show that the relative strength of this channel and its contribution to the THz conductivity are, however, still an open question. The similarity between THz (few meV) and mid-IR pump implies that this channel is relatively weak for THz and mid-IR pumping when compared to the intraband excitation channel, unlike in the case of optical pump, which warrants further studies. In addition, our ﬁtting is faithful because it only needs to change two parameters, which are the two time-dependent scattering rates directly seen in distinctly different time-resolved THz lineshapes. Since the ﬁtting result is already uniquely converging with the two ﬁtting parameters, additional parameters only relax the constraint and add uncertainty, which is hard to be physically meaningful. The mid-IR/THz pump spectroscopy experiment like ours reveals ultrafast manipulation of surface and bulk THz conductivity via wavelength-selective pumping and underpin the difference of intraband vs. interband pumping, shown in Fig.5, without reference to any model and/or assumption forﬁtting. The observation of frequency-dependent hot carrier cooling times is shown in Fig. 2a–d, which directly distinguish the faster surface channel from the slower bulk in the raw data. These ultrafast conductivity dynamics of surface states are absent in the prior static THz and time-averaged probes.

Finally, we note that the assignment of THz conductivity of these two decay channels is justiﬁed by the distinctly different THz spectrum lineshapes and dynamics of the surface and bulk states,

**a** _{b}

4

3

2

1

0

–

Δ

*E*sampl

e

(

a

.u.)

200 100 0

Δ*t*pp(ps) Δ*t*pp(ps)
7 μJ cm–2

3.5 μJ cm–2

1.6 μJ cm–2

390 meV pump

*T *= 5 K

200 100 0

248 meV pump

*T *= 5 K
19 μJ cm–2

9.5 μJ cm–2 7 μJ cm–2 390 meV,1.6 μJ cm–2

Fig. 6Ultrafast THz dynamics under interband and intraband

photoexcitations. Pump-induced THzﬁeld changesΔEsampleas a function of

pump-probe delayΔtppaftera390 meV (3.18μm) andb248 meV (5μm)

photoexcitations at variousﬂuences andT=5 K. The gate timetgateisﬁxed

at the peak of the static THzﬁeld shown in Fig.1d. One of the THz traces
froma(pink curve, 1.6_{μ}J cm−2) is also plotted inbas a_{ﬁ}lled gray curve for
better comparison

respectively. First, only the TI surface state could give rise to a photoexcited negative THz conductivity in Fig. 2e and intraband decay of Dirac spectrum at the surface is much faster than the bulk. Second, the other channel, i.e., photoexcited positive THz con-ductivity that we have assigned to bulk in Fig.2f, exhibits a decrease in the scattering rate. This is well explained by the reduced ionized impurity scattering which leads to a decrease in scattering rate and an increase in THz conductivity at low frequency after photo-excitation. Third, a decrease in Bi2Se3thickness has been shown to

induce a transition from a bulk-like, positive conductivity to a surface-like, negative THz conductivity30.

In conclusion, we have provided the measurement and insights
into the intraband, mid-IR, and THz pump-induced quantum
transport in TIs. We achieve this by suppressing all interband
transitions that mask the processes of main interest. The
con-clusions from this advanced spectroscopy are the demonstration
of another tuning knob for both controlling THz conductivity
and isolating the surface contribution from the bulk contribution,
by using low photon energy pumping and comparing them to
optical pumping. This scheme enables a clear observation of
enhanced surface transport, which provides evidence for helical
spin structure of surface (Dirac) electrons that suppresses
back-scattering. The pump photon energy tuning achieved in this way
also allows us to control the surface transport optically in a
selective way. Our experiments may evolve into a benchmark
characterization method for high frequency topological transport
in TI-based device development, and motivate fundamental
quantum phase discovery and control at the boundaries of
topology, magnetism34_{, and other broken symmetry states}35–37_{.}

Methods

Experimental schemes. Our mid-IR/THz pump and THz probe spectrometer is

driven by a 1 kHz Ti:sapphire regenerative ampliﬁer, which has 800 nm central
wavelength and 40 fs pulse duration38_{. The majority of the output is used to}

pump either an optical parametric ampliﬁer to generate mid-IR pulses tunable
from 3–15μm (or 83–413 meV) or a lithium niobate crystal to generate strong THz
pulses centered at 4 meV39_{allowing for selective intraband and interband }

photo-excitation. The other part of the output is used to generate and detect phase-locked THz electricﬁelds in time-domain via optical rectiﬁcation and electro-optic sam-pling in a 1 mm thick ZnTe crystal, respectively. THzﬁelds with a bandwidth from 0.5 to 2.5 THz (2.1–10.3 meV) are used as a probe beam. The measurement scheme is brieﬂy illustrated in Fig.1a, in which mid-IR (red) or THz (yellow) pump photoexcites the sample and THz pulse (light blue) probes photoinduced responses of the sample. The transmitted THz probe containing spectral amplitude and phase information of the sample is directly measured in time-domain using an optical gate pulse. The setup is enclosed in a N2gas purge box.

Sample preparation and characterization. The Bi2Se3thinﬁlm sample, 50 nm

thick, is grown by molecular beam epitaxy on a 0.5 mm thick sapphire substrate. The sample is mounted together with a 0.5 mm thick pure sapphire substrate, used as a reference, into a cryostat with temperatures down toT=5 K. Two copper mounts with the same aperture are placed directly in front of the sample and reference to ensure uniform photoexcitation and accurate comparison of their THz transmission.

The sample studied has a Fermi energyEF~ 60 meV from the bulk conduction

band edge (Fig.1a), as estimated from the measured plasma frequency in the static THz conductivity spectra shown in Fig.1b. The gray lines are theoreticalﬁttings that are discussed in Results. The estimated Fermi energy is consistent with the difference between the separately measured, interband optical transition onset

Einter~ 390 meV using our wavelength-dependent pump-induced THzﬁeld change

data (see Supplementary Note 1) and the bulk insulating bandgapEg~ 332 meV,

which yields a similarEF=Einter−Eg~ 58 meV. Please note that the exact value of

the gap size is not critical for our scheme, nor does it change our conclusion, as long as the interband transition gap in our sample is larger than our pump photon energy, e.g., 4 meV and 248 meV used.

THz data analysis. Raw THzﬁeld transients are measured as a function of gate

timetgateafter transmission through (i) the reference bare substrateEref(tgate), (ii)

the unexcited sampleEsample(tgate), and (iii) as pump-induced changeΔEsample

(tgate,Δtpp) at pump-probe delayΔtpp. Figure1c,d shows the 2D false-color plots of

ΔEsample(tgate,Δtpp) after below gap photoexcitation at 248 meV (5μm) for high

(300 K) and low (5 K) temperatures, respectively. Also plotted in the aboveﬁgures are the correspondingEsample(tgate) (green curves) and pump-induced change

ΔEsample(tgate) atΔtpp=1 ps (blue curves). For the unexcited sample, through the

fast Fourier transformation and Fresnel equation, the static THz conductivity, shown in Fig.1b, is directly obtained from the experimentally measured complex transmission coefﬁcient~tðωÞwith spectral amplitude and phase information extracted by comparing theﬁelds transmitted through sample and reference, i.e.,

~

tðωÞ ¼EsampleðωÞ=ErefðωÞ, similar to the method reported in ref.29(see also

Supplementary Note 5). For the excited sample atΔtpp, the complex transmission

coefﬁcient is obtained by~texcitedðωÞ ¼ ½ΔEsampleðωÞ þEsampleðωÞ=ErefðωÞand is

used to extract the photoexcited transient THz conductivity. Afterwards, the pump-induced conductivity changeΔσ~ðωÞ ¼~σexcitedðωÞ ~σðωÞis calculated. The

corresponding dielectric function can be calculated by the equation

~

σðωÞ ¼i½1~εðωÞωε0. The simultaneously obtained real parts of transient

con-ductivity changeΔσ1(ω) and dielectric function changeΔε1(ω) as a function ofΔtpp

are presented in the study, which allow us to quantitatively describe the ultrafast dynamic evolution of the photoexcited Dirac and bulk fermions and their intrinsic scattering processes.

Data availability

The data that support theﬁndings of this study are available from the corresponding author upon reasonable request.

Received: 28 April 2018 Accepted: 18 January 2019

References

1. Hsieh, D. et al. A topological Dirac insulator in a quantum spin Hall phase.

Nature452, 970 (2008).

2. Zhang, H. et al. Topological insulators in Bi2Se3, Bi2Te3and Sb2Te3with a

single Dirac cone on the surface.Nat. Phys.5, 438 (2009).

3. Moore, J. E. The birth of topological insulators.Nature464, 194 (2010). 4. Hasan, M. Z. & Kane, C. L. Colloquium: topological insulators.Rev. Mod.

Phys.82, 3045 (2010).

5. Qi, X.-L. & Zhang, S.-C. The quantum spin Hall effect and topological insulators.Phys. Today63, 33 (2010).

6. Koirala, N. et al. Record surface state mobility and quantum hall effect in topological insulator thinﬁlms via interface engineering.Nano. Lett.15, 8245 (2015).

7. Bowlan, P. et al. Probing and controlling terahertz-driven structural dynamics with surface sensitivity.Optica4, 383 (2017).

8. Hsieh, D. et al. A tunable topological insulator in the spin helical Dirac transport regime.Nature460, 1101 (2009).

9. Wu, C., Bernevig, B. A. & Zhang, S.-C. Helical liquid and the edge of quantum spin hall systems.Phys. Rev. Lett.96, 106401 (2006).

10. Kane, C. L. & Mele, E. J. Z2topological order and the quantum.Phys. Rev.

Lett.95, 146802 (2005).

11. Moore, J. E. & Balents, L. Topological invariants of time-reversal-invariant band structures.Phys. Rev. B75, 121306(R) (2007).

12. Zyuzin, A. A. & Burkov, A. A. Topological response in Weyl semimetals and the chiral anomaly.Phys. Rev. B86, 115133 (2012).

13. Bravyi, S., Hastings, M. B. & Verstraete, F. Lieb-Robinson bounds and the generation of correlations and topological quantum order.Phys. Rev. Lett.97, 050401 (2006).

14. Qu, D.-X., Hor, Y. S., Xiong, J., Cava, R. J. & Ong, N. P. Quantum oscillations and hall anomaly of surface states in the topological insulator Bi2Te3.Science 329, 821 (2010).

15. Wang, Y. H. et al. Measurement of intrinsic dirac fermion cooling on the surface of the topological insulator Bi2Te3using time-resolved and

angle-resolved photoemission spectroscopy.Phys. Rev. Lett.109, 127401 (2012).

16. Sobota, J. A. et al. Ultrafast optical excitation of a persistent surface-state population in the topological insulator Bi2Se3.Phys. Rev. Lett.108, 117403

(2012).

17. Giorgianni, F. et al. Strong nonlinear terahertz response induced by Dirac surface states in Bi2Se3topological insulator.Nat. Commun.7, 11421 (2016).

18. Kuroda, K., Reimann, J., Güdde, J. & Höfer, U. Generation of transient photocurrents in the topological surface state of Sb2Te3by direct optical

excitation with midinfrared pulses.Phys. Rev. Lett.116, 076801 (2016). 19. Iyer, V., Chen, Y. P. & Xu, X. Ultrafast surface state spin-carrier dynamics in

the topological insulator Bi2Te2Se.Phys. Rev. Lett.121, 026807 (2018).

20. Valdés Aguilar, R. et al. Terahertz response and colossal Kerr rotation from the surface states of the topological insulator Bi2Se3.Phys. Rev. Lett.108,

087403 (2012).

21. Wu, L. et al. Quantized Faraday and Kerr rotation and axion electrodynamics of a 3D topological insulator.Science354, 1124 (2016).

### ARTICLE

NATURE COMMUNICATIONS | https://doi.org/10.1038/s41467-019-08559-622. Zhang, Y. et al. Crossover of the three-dimensional topological insulator Bi2Te3to the two-dimensional limit.Nat. Phys.6, 584 (2010).

23. Linder, J., Yokoyama, T. & Sudbø, A. Anomalousﬁnite size effects on surface states in the topological insulator Bi2Te3.Phys. Rev. B80, 205401 (2009).

24. Liu, C.-X. et al. Oscillatory crossover from two-dimensional to three-dimensional topological insulators.Phys. Rev. B81, 041307(R) (2010). 25. Lu, H.-Z., Shan, W.-Y., Yao, W., Niu, Q. & Shen, S.-Q. Massive Dirac fermions

and spin physics in an ultrathinﬁlm of topological insulator.Phys. Rev. B81, 115407 (2010).

26. Okada, K. N. et al. Terahertz spectroscopy on Faraday and Kerr rotations in a quantum anomalous Hall state.Nat. Commun.7, 12245 (2016).

27. Dziom, V. et al. Observation of the universal magnetoelectric effect in a 3D topological insulator.Nat. Commun.8, 15197 (2017).

28. Valdés Aguilar, R. et al. Time-resolved terahertz dynamics in thinﬁlms of the topological insulator Bi2Se3.Appl. Phys. Lett.106, 011901 (2015).

29. Wu, L. et al. A sudden collapse in the transport lifetime across the topological phase transition in (Bi1−xInx)2Se3.Nat. Phys.9, 410 (2013).

30. Sim, S. et al. Ultrafast terahertz dynamics of hot Dirac-electron surface scattering in the topological insulator Bi2Se3.Phys. Rev. B89, 165137 (2014).

31. Ozturk, T. et al. Inﬂuence of helical spin structure on the magnetoresistance of an ideal topological insulator.J. Phys. Commun.1, 035005 (2017). 32. Yan, B. & Felser, C. Topological materials: Weyl semimetals.Annu. Rev.

Condens. Matter Phys.8, 337 (2017).

33. Chattopadhyay, D. & Queisser, H. J. Electron scattering by ionized impurities in semiconductors.Rev. Mod. Phys.53, 745 (1981).

34. Wang, J. et al. Ultrafast softening in InMnAs.Phys. E20, 412 (2004). 35. Yang, X. et al. Non-equilibrium pair breaking in Ba(Fe1−xCox)2As2

superconductors: evidence for formation of photo-induced excitonic spin-density-wave state.Phys. Rev. Lett.121, 267001 (2018).

36. Patz, A. et al. Critical speeding up of nonequilibrium electronic relaxation near nematic phase transition in unstrained Ba(Fe1−xCox)2As2.Phys. Rev. B95,

165122 (2017).

37. Patz, A. et al. Ultrafast observation of critical nematicﬂuctuations and giant magnetoelastic coupling in iron pnictides.Nat. Commun.5, 3229 (2014).

38. Luo, L., Chatzakis, I., Patz, A. & Wang, J. Ultrafast terahertz probes of interacting dark excitons in chirality-speciﬁc semiconducting single-walled carbon nanotubes.Phys. Rev. Lett.114, 107402 (2015).

39. Yang, X. et al. Terahertz-light quantum tuning of a metastable emergent phase hidden by superconductivity.Nat. Mater.17, 586 (2018).

Acknowledgements

This work was supported by the U.S. Department of Energy, Ofﬁce of Basic Energy Science, Division of Materials Sciences and Engineering (Ames Laboratory is operated for

the U.S. Department of Energy by Iowa State University under Contract No. DE-AC02-07CH11358) (science driver, THz spectroscopy experiment and theory). Sample devel-opment was supported by National Science Foundation DMR 1400432. Terahertz spectroscopy instrument was supported in part by National Science Foundation EECS 1611454. Additional analysis by I.E.P and M.M was supported by the U.S. Department of Energy, Ofﬁce of Science, Basic Energy Sciences under Award #DE-SC0019137.

Author contributions

L.L. and X.Y. performed the experimental measurements and collected the data. They analysed the results and developed the model with the help of J.W., Z.L., C.V., D.C., M.M., X.Z., Y.Y., C.Z.W., K.M.H. and I.E.P. Thinﬁlm growth and basic characterizations are done by X.L., M.D. and J.K.F. at University of Notre Dame. J.W. and L.L. wrote the paper with help from all authors. J.W. supervised the study.

Additional information

Supplementary Informationaccompanies this paper at https://doi.org/10.1038/s41467-019-08559-6.

Competing interests:The authors declare no competing interests.

Reprints and permissioninformation is available online athttp://npg.nature.com/ reprintsandpermissions/

Journal peer review information:Nature Communicationsthanks the anonymous reviewers for their contribution to the peer review of this work.

Publisher’s note:Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional afﬁliations.

Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visithttp://creativecommons.org/ licenses/by/4.0/.

© The Author(s) 2019